<i>M</i>Yb(BH~4~)~4~ (<i>M</i> = K, Na) from laboratory X-ray powder data
Wegner, Wojciech; Jaroń, Tomasz; Grochala, Wojciech; Acta Crystallographica Section C 69 (2013) 1289–1291; doi:10.1107/S0108270113027145

data_2019203
_publ_section_title
;
 <i>M</i>Yb(BH~4~)~4~ (<i>M</i> = K, Na) from laboratory X-ray powder data
;
_journal_coeditor_code           CU3040
_journal_issue                   11
_journal_name_full               'Acta Crystallographica Section C'
_journal_page_first              1289
_journal_page_last               1291
_journal_paper_doi               10.1107/S0108270113027145
_journal_volume                  69
_journal_year                    2013
_chemical_formula_iupac          'K Yb (B H4)4'
_chemical_formula_moiety         'B4 H16 Yb, K'
_chemical_formula_sum            'B4 H16 K Yb'
_chemical_formula_weight         271.5
_chemical_name_systematic
;
Potassium ytterbium tetraborohydride
;
_space_group_IT_number           63
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   8.4341(13)
_cell_length_b                   12.445(2)
_cell_length_c                   9.6449(15)
_cell_measurement_temperature    293
_cell_volume                     1012.4(3)
_computing_cell_refinement
'JANA2006 (Pet\<r\'i\<cek <i>et al.</i>, 2006)'
_computing_data_collection       'DIFFRACplus (Bruker, 2006)'
_computing_data_reduction        'DIFFRACplus (Bruker, 2006)'
_computing_molecular_graphics    'VESTA (Momma & Izumi, 2011)'
_computing_publication_material  'publCIF (Westrip, 2010)'
_computing_structure_refinement
'JANA2006 (Pet\<r\'i\<cek <i>et al.</i>, 2006)'
_computing_structure_solution
'JANA2006 (Pet\<r\'i\<cek <i>et al.</i>, 2006)'
_diffrn_ambient_temperature      293
_diffrn_measurement_device_type  'Bruker D8 Discover'
_diffrn_radiation_type           'Cu K\a'
_diffrn_radiation_wavelength     1.5418
_exptl_absorpt_coefficient_mu    19.984
_exptl_crystal_density_diffrn    1.7808
_exptl_crystal_F_000             80
_pd_char_colour                  green
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        110.009
_pd_meas_2theta_range_min        10.000
_pd_meas_number_of_points        4889
_pd_meas_scan_method             cont
_pd_proc_2theta_range_inc        0.02
_pd_proc_2theta_range_max        110.009
_pd_proc_2theta_range_min        10
_pd_proc_ls_background_function  '30 Legendre polynomials'
_pd_proc_ls_pref_orient_corr     none
_pd_proc_ls_profile_function     pseudo-Voigt
_pd_proc_ls_prof_R_factor        0.0052
_pd_proc_ls_prof_wR_expected     0.0055
_pd_proc_ls_prof_wR_factor       0.0073
_pd_spec_mounting                'quartz capillary'
_pd_spec_mount_mode              transmission
_pd_spec_shape                   cylinder
_pd_spec_size_axial              18
_pd_spec_size_equat              0.3
_refine_diff_density_max         0.18
_refine_diff_density_min         -0.24
_refine_ls_goodness_of_fit_all   1.32
_refine_ls_hydrogen_treatment    refall
_refine_ls_number_constraints    7
_refine_ls_number_parameters     71
_refine_ls_number_restraints     23
_refine_ls_R_factor_all          0.0204
_refine_ls_R_factor_gt           0.0204
_refine_ls_shift/su_max          0.0441
_refine_ls_shift/su_mean         0.0054
_refine_ls_weighting_details     'w = 1/[\s^2^(I)+0.0016I^2^]'
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_all         0.0235
_refine_ls_wR_factor_gt          0.0235
_cod_data_source_file            cu3040.cif
_cod_data_source_block           I
_cod_database_code               2019203